Dear Label_Name,

Greetings! I hope you are well.

I am writing on behalf of an international publishing house, Science and Education Publishing, USA (http://www.sciepub.com).

Science and Education Publishing (SciEP) is a multidisciplinary open access publisher of Journals covering the fields of Science, Technology and Medicine. All SciEP publications are subject to high-quality peer review, editorial and production processes and are freely available online.

Welcome to the April, 2013 edition of SciEP newsletter, providing monthly summaries of articles on science & education related topics of interest to scientist and professionals. The mission of our journals is to provide an open access forum for publishing new findings on issues pertinent to scientific and academic field. We also invite you to submit original research papers, review articles, short reports, or case studies are considered for publication in our Multidisciplinary Journals.

American Journal of Public Health Research
DOI: 10.12691/ajphr-1-1-3

The Implementation of a Tele-Homecare System with Service Oriented Architecture and HL7 Message Transmission Standard
Ching-Sung Wang

American Journal of Medical and Biological Research
DOI: 10.12691/ajmbr-1-1-2

The Influence of Ethanol on Pyruvate Kinases Activity in Vivo, in Vitro, in Silico
Lelevich Sergey Vladimirovich, Khrustalev Vladislav Victorovich, Barkovsky Eugene Victorovich, Shedogubova Tatyana Aleksandrovna

American Journal of Medical Sciences and Medicine
DOI: 10.12691/ajmsm-1-1-1

Clinical and Histological Features in Wegener Granulomatosis
Li Cavoli Gioacchino, Passantino Rita, Bono Luisa, Tortorici Calogera, Ferrantelli Angelo, Giammarresi Carlo, Rotolo Ugo

American Journal of Infectious Diseases and Microbiology
DOI: 10.12691/ajidm-1-1-2

The Curse of Lymphatic Filariasis: Would the Continual Use of Diethylcarbamazine Eliminate this Scourge in Papua New Guinea?
Anne Lanham, Lillian Mwanri

We have released issues of some journals on February 2013.
American Journal of Public Health Research
American Journal of Medical Sciences and Medicine
American Journal of Medical and Biological Research
American Journal of Pharmacological Sciences
American Journal of Clinical Medicine Research
American Journal of Nursing Research
American Journal of Cancer Prevention
American Journal of Medicine Studies
American Journal of Infectious Diseases and Microbiology
American Journal of Cardiovascular Disease Research
American Journal of Biomedical Research
American Journal of Mechanical Engineering
American Journal of Microbiological Research
Journal of Preventive Medicine
American Journal of Food and Nutrition
American Journal of Hypertension Research
American Journal of Sports Science and Medicine
Journal of Cancer Research and Treatment
American Journal of Zoological Research
Journal of Biomedical Engineering and Technology
American Journal of Microbiological Research
Biomedical Science and Engineering

We are pleased to announce that submissions are now being accepted for peer review for all the journals across all our subject areas in SciEP.

Please submit your manuscript via our online submission system:
http://www.sciepub.com/author/signin

To unsubscribe from our mailing list, please click on the following link: unsubscribe

I am looking forward to hearing from you.

Kind regards,

David Rain
Email:join@sciepub.com
Science and Education Publishing (http://www.sciepub.com)

Microwave Assisted Green Synthesis, Characterisation of Alanine Templated Aluminophosphate Zeolite and Study of Its Application as Adsorbent

Shalini K S, Nirmala B*

Department of Chemistry, Tumkur University, Tumkur, Karnataka, India

Abstract: The present work is concerned with synthesis of aluminophosphate zeolites with tridymit framework by employing microwave technique and alanine as structure directing agent. Aluminophosphate zeolite was characterised using XRD, SEM- EDAX, BET and FTIR. Adsorption efficiency of the synthesised aluminophosphate zeolite was evaluated using water soluble dye methylene blue as a model pollutant. Influence of pH, Adsorbent dosage, Dye concentration and contact time were studied. Experimental data fitted well with pseudo bimolecular kinetic model and freundlich’s adsorption isotherm (R²=1) with yielding a maximum adsorption capacity of 37.016ppm mg⁻¹.

Keywords: microwave synthesis, aluminophosphate, methylene blue, adsorption studies

Received October 20, 2019; Revised November 21, 2019; Accepted December 02, 2019

Citation: Shalini K S, Nirmala B, Microwave Assisted Green Synthesis, Characterisation of Alanine Templated Aluminophosphate Zeolite and Study of Its Application as Adsorbent. Applied Ecology and Environmental Sciences, 7 (6). 231-237. January 2019. doi:10.12691/aees-7-6-4

1. Introduction

Unusual physicochemical properties of zeolites and zeolite like frameworks such as Silicates, aluminosilicates, aluminophosphates and metal substituted aluminophosphate zeolites play a significant role in augmenting their industrial applications mainly as adsorbents, catalysts and in membrane separation [1,2,3]. Aluminophosphates specifically are important members of this family as they have silicon free composition but are also similar to zeolites in morphology and function.

Microporous nature of aluminophosphates retards the rate of diffusion on to molecular sieves there by reducing the efficiency of the molecules as adsorbents, catalysts or membrane separation. Synthesis of mesoporous aluminophosphate with ordered structure will enhance diffusion of reactants on to zeolite frameworks [4]. Intensive research is being carried out in this field of designing and synthesis of aluminophosphates with desired structural and physicochemical properties for specific applications by altering various synthetic parameters such as Aluminium phosphate ratio, by using different structure directing agents such as surfactants, quaternary ammonium salts, amines, organosilanes etc., changing synthesis conditions like Ionothermal synthesis [5], hydrothermal synthesis [6], Solvothermal synthesis [7], vapour phase synthesis [8], solvent free synthesis [9] etc. Combinatorial methods are being employed for the synthesis of aluminophosphate zeolites [10] conventional techniques involve High temperature and pressure along with long reaction times.

Water soluble dyes or colouring agents such as Methylene blue, Malachite green, trypan blue, Evan’s Blue, sulphur dyes etc., are used extensively in many industries such as paper, pulp, leather, textiles and hence are major threat to environmental safety, particularly to our water bodies. With growing awareness about environment and its wellbeing massive research work is being done worldwide in developing materials and techniques to aid in removing these pollutants from water bodies. Although various techniques both physicochemical and biological techniques such as flocculation [11], precipitation, coagulation, ozonation, photo degradation, membrane filtration are available, it has been found tough to remove organic dyes and pigments using conventional methods owing to their complex structures and stability towards action of light or oxidizing agents and resistance to aerobic digestion. Adsorption is one of the favourable techniques for removing water soluble dyes [12] and Aluminophosphate zeolites are promising materials in removal of these water soluble dyes by adsorption.

Microwave assisted synthesis of aluminophosphates offers the advantage of quick synthesis of aluminophosphates under normal temperature and pressure [5,13,14,15]. Current study gives a brief account of synthesis of Aluminophosphate with tridymit framework employing microwave assisted synthetic technique and amino acids as structure directing agents. Structure and morphology of aluminophosphates were studied using XRD, IR, SEM-EDAX and BET. Adsorption capacity of the synthesised aluminophosphates in removing water soluble dyes was evaluated using Methylene Blue as model adsorbent.

2. Materials and Methods

2.1. Synthesis

Aluminium Hydroxide (LR grade) used as source of Aluminium, Ortho phosphoric acid (LR grade) used as source of Phosphorus and (±) alanine(LR grade) was used as structure directing agent for the synthesis of aluminophosphates. Methylene Blue (LR grade) was used to evaluate adsorption capacity of AlPOs.

3.9g (1mmol) of Aluminium hydroxide was dispersed in 10mL of distilled water and stirred for 15 min. 5.6mL (2mmol) of orthophosphoric acid was added dropwise to the dispersion with constant stirring. Reaction mixture was stirred for 1h at room temperature. 2.22g (0.05mmol) of Alanine was dissolved in 10mL of distilled water and added to the reaction mixture with constant stirring. The gel was aged for 1h at room temperature and subjected to microwave irradiation (160W, 20 min) after noting the Initial and Final pH. White precipitate of Aluminophosphates formed was washed thoroughly with distilled water under ultra-sonication. The product was then filtered and dried in hot air oven at 200°C for 2h.

2.2. Characterization

Phase purity of the synthesised Aluminophosphates was examined using powder x-ray diffraction pattern (XRD smart lab x-ray diffratometer (CuK α , λ=1.5406 å). FTIR spectra of the particles give an understanding in to the nature of bonding. Details pertaining to surface morphology, elemental composition and crystal size were obtained using SEM with EDAX (VEGA 3 TESCAN). Surface area was determined using Quatachrome instruments-Nova station 0, version 3. Adsorption studies with respect to methylene blue were studied using colorimeter.

2.3. Adsorption Studies

Batch sorption experiments were conducted to evaluate the effect of various factors such as pH, adsorbent dosage, initial dye concentration, contact time [16,17,18].

2.4. Effect of pH

100ml of 5ppm methylene blue solution was adjusted to different initial pH values (pH 3, 5, 7, 9 and 11). The solutions were then stirred with 5mg of adsorbent. 2ml of the solution was withdrawn at regular intervals, centrifuged and absorbance of the centrifugate was measured. Percentage of adsorption was calculated using eq. 1.

[picture] | (1)

2.5. Effect of Adsorbent Dosage

100ml of 5ppm methylene blue solution was stirred with different amount of adsorbent (5, 10, 15, 20, 25 mg). 2ml of dye solution was withdrawn at regular interval of time and absorbance was measured after removing catalyst by centrifugation. Percentage of adsorption was calculated using eq. 1.

2.6. Effect of Initial Dye Concentration

100ml of dye solution of varying concentrations (1, 2, 3, 4, 5ppm) was stirred with 10mg of adsorbent. Dye solution was withdrawn at regular interval of time, centrifuged and absorbance of centrifugate was measured. Percentage of adsorption was calculated using eq.1.

The results obtained were analysed using kinetic models and adsorption isotherms to understand the nature of adsorption of methylene blue by aluminophosphate zeolites.

3. Results and Discussions

X-Ray diffraction pattern of Ala templated alumminophosphates presented in Figure 1a. All the peaks in the diffraction pattern of the obtained compound can be indexed as belonging to ALPO₄-tridymit (orthorhombic) phase (a= b= 7.082 and c= 6.993) corresponding to JCPDS no-11-500. Average particle size D calculated using Debye- Scherrer equation (2) [19],

[picture] | (2)

Willamson–Hall (W-H) method was used to calculate the lattice strain from the following modified Scherrer equation (3) [19],

[picture] | (3)

W-H plot of βcosθ against 4sinθ is shown in Figure 1b. Dislocation density (δ) is estimated using the below equation (4), the calculated physical parameters are given in Table 1.

[picture] | (4)

Table 1. Physical parameters of ala templated Aluminophosphate zeolites

Figure 1.(a) PXRD pattern of ALPO-tridymit (b) W-H plot

Figure 2. SEM image of Aluminophosphate zeolites

Figure 3. EDAX of Aluminophosphate zeolites

SEM images of synthesized Aluminophosphate zeolites are given in Figure 2 and from the image it is evident that the particles have a spherical morphology and EDAX (Figure 3) confirms the purity of the synthesized Aluminophosphate zeolites.

Surface area and Pore size analysis: Nitrogen adsorption, desorption isotherms of Aluminophosphates (Figure 4a) shows no typical hysteresis indicating the presence of blind cylindrical, cone shaped or wedge shaped pores (Figure 4a) [20].

A linear plot of [1/W ((Po/P)-1)] vs P/Po presented in Figure 4b. The surface area of the aluminophosphates was found to be 2.743m²/g. From nitrogen desorption isotherm using BJH analysis, pore volume and pore radius were determined and found to be 0.004cm³/g and 19.2Ǻ respectively (Figure 4c). Hence synthesized aluminophosphates can be considered to be mesoporous in nature [21].

Infrared spectroscopy: FTIR spectrum of Aluminophosphate zeolites shown in Figure 5. Peaks around 468-545cm⁻¹ corresponds to bending vibrations of PO₄, Sharp peak at 615 cm⁻¹ can be attributed to interaction between alumina and Al³⁺. Symmetric stretching of PO₄ tetrahedra is confirmed by sharp peaks in the region 700-740cm⁻¹. Characteristic peak of PO₄ tetrahedra is observed at 1115 cm⁻¹. Broad band in the region 3000-3100cm⁻¹ corresponds to the presence of surface hydroxyl groups [21].

Figure 4. (a) adsorption desorption isotherm (b) multipoint BET analysis (c) BJH Pore diameter analysis

Figure 5. FTIR spectra of Aluminophosphate zeolite

4. Adsorption studies of Methylene Blue on to Aluminophosphates

Methylene blue was used as a model dye to study the effectiveness of aluminophosphate zeolites as adsorbents. From Figure 6 it is evident that adsorption is maximum at pH 7. Adsorption attains equilibrium with in initial 20 minutes irrespective of adsorbent dosage and initial dye concentrations (Figure 7 and Figure 8). Aluminophosphate zeolites were found to be more effective as adsorbents at lower dosages but efficiency decreases with increasing dosage. This is due to blocking of pores on zeolite surface due to aggregation of adsorbents with increased concentration. A compilation of previous results of methylene blue adsorption from literature is given in Table 2.

Figure 6. Effect of pH on adsorption of Methylene blue

Figure 7. Effect of adsorbent dosage on adsorption of Methylene blue

Figure 8. Effect of Initial dye concentration on adsorption to adsorbents

Table 2. Comparison of adsorption of methylene blue on ALPOs with reported results

Decrease in adsorption efficiency can be attributed to low surface area of ala templated aluminophosphate zeolites and also to the blind pores in the adsorbent.

Figure 9. Plot of t/ qt vs time in minutes.

Figure 10. (a) Langmuir’s adsorption isotherm (b) Freundlich’s adsorption isotherm

Table 3. Parameters of Kinetics and adsorption isotherms for adsorption of methylene blue

Kinetic parameter data presented in Table 3 confirms that the process of adsorption follows pseudo bimolecular kinetics. In this model, rate of adsorption depends on the amount of dye adsorbed on to the surface of adsorbent and to the amount adsorbed at equilibrium. A plot of t/qt vs time in minutes gives a straight line graph with pearson correlation coefficient R2 value equal to 0.9697 (Figure 9). From the plot, rate of adsorption was found to be 7.21 x 10² ppm mg⁻¹ min⁻¹. It also implies that the adsorption process is a multilayer process which is augmented by the results of study of adsorption isotherm models. A plot of Ce/qe vs Ce (Langmuir’s isotherm) and –logCe vs –log qe (Freundlich’s Isotherm) were presented in Figure 10 (a) and (b) respectively. From the two plots, it can be derived that plot of –logCe vs –log qe gives a straight line graph with slope 1/n and intercept –log Kf. Adsorption process fits well with freundlich’s adsorption model of multilayer adsorption as suggested by pearson correlation factor which was calculated to be 1 and dimensional quantity n which corresponds to intensity of adsorption was determined to be 1 indicating that the process of adsorption is moderate [26]. Adsorption of methylene blue on to Aluminophosphate zeolite follows freundlich adsorption isotherm indicating a multilayer adsorption process (Figure 10) [16,17]. Experimental parameters corresponding to Kinetic study and adsorption isotherm study of adsorption of methylene blue on ala templated aluminophosphate are presented in Table 3 [24].

5. Conclusion

Aluminophosphates with orthorhombic phase was synthesized using alanine as structure directing agent under ambient conditions. Scanning electron microscope images confirm aggregates of roughly spherical plate like structures with dimensions in the range of 230nm. Surface area of Aluminophosphates was found to be 2.743m²/g and pore radius 19.2Ǻ. Adsorption of methylene blue by amino acid templated aluminophosphates follows pseudo second order kinetics with rate 7.21 x102 ppm mg⁻¹min⁻¹ and follows freundlich adsorption isotherm indicating a multilayer process.

Acknowledgement

Authors are grateful to STIC, Cochin for providing instrumentation facilities for characterization.

References

[1]   | Y. Wang, X. Zou, L. Sun, H. Rong and G. Zhu, “A zeolite-like Aluminophosphate membrane with molecular seiving property foe water desalination,” Chemical Science, vol. 9, pp. 2533-2539, 7 March 2018.
[2]   | Y. Li, L. Li and J. Yu, “Applications of Zeolites in Sustainable Chemistry,” Chem, vol. 3, no. 6, pp. 928-949, 2017.
[3]   | X.-Y. Yang, L.-H. Chen, Y. Li, J. C. Rooke, C. Sanchez and B.-L. Su, “Hierarchically porous materials: synthesis strategies and structure design,” Chemical Society Reviews, vol. 46, no. 2, pp. 481-558, 2017.
[4]   | Z. Liu, Y. Hua, J. Wang, X. Dong, Q. Tian and Y. Han, “Recent progress in the direct synthesis of hierarchical zeolites: synthetic strategies and characterization methods,” Materials Chemistry Frontiers, vol. 1, no. 11, pp. 2195- 2212, 2017.
[5]   | Y.-P. Xu, Z.-J. Tian, S.-J. Wang, Y. Hu, L. Wang, B.-C. Wang, Y.-C. Ma, L. Hou, J.-Y. Yu and L.-W. Lin, “Microwave-Enhanced Ionothermal Synthesis of Aluminophosphate Molecular Sieves,” Angewandte Chemie International Edition, vol. 45, no. 24, pp. 3965-3970, 2006.
[6]   | T. Ban, S. Iriyama and Y. Ohya, “Bottom-up synthesis of aluminophosphate nanosheets by hydrothermal process,” Advanced Powder Technology, vol. 29, no. 3, pp. 537-542, 2018.
[7]   | Z.-Z. Bao, A.-H. Sun, S.-D. Han, J.-H. Li, G.-M. Wang and Z.-H. Wang, “Aluminophosphates prepared using in situ generated tetramethylammonium cations as structure directing agents,,” Solid State Sciences,, vol. 61, pp. 77-83, 2016.
[8]   | S. Thoma and T. Nenoff, “Vapor phase transport synthesis of zeolites from sol–gel precursors,” Microporous and Mesoporous Materials, vol. 41, no. 1-3, pp. 295-305, 2000.
[9]   | N. Sheng, Y. Chu, S. Xin, Q. Wang, X. Yi, Z. Feng, X. Meng, X. Liu, F. Deng and F.-S. Xiao, “Insights of the Crystallization Process of Molecular Sieve AlPO4-5 Prepared by Solvent-Free Synthesis,” Journal of the American Chemical Society, vol. 138, no. 19, pp. 6171-6176, 2016.
[10]   | K. Choi, D. Gardner, N. Hilbrandt and T. Bein, “Combinatorial Methods for the Synthesis of Aluminophosphate Molecular Sieves,” Angewandte Chemie International Edition, vol. 38, no. 19, pp. 2891-2894, 1999.
[11]   | M. O. Agunbiade, E. Van Heerden, C. H. Pohl and A. T. Ashafa, “Flocculating performance of a bioflocculant produced by Arthrobacter humicola in sewage waste water treatment,” BMC Biotechnology, vol. 17, no. 1, pp. 51-59, 2017.
[12]   | S. Selvaraju and B. L. GRACE, “Removal of Dyes from Wastewater using Adsorption -A Review,” International journal of biosciences and technology, vol. 2, no. 4, pp. 47-51, 2009.
[13]   | R. Martínez-Palou, “Microwave-assisted synthesis using ionic liquids,” Molecular Diversity, vol. 14, no. 1, pp. 3-25, 2010.
[14]   | Z. Liu, J. Zhu, T. Wakihara and T. Okubo, “Ultrafast synthesis of zeolites: breakthrough, progress and perspective,” Inorganic Chemistry Frontiers, vol. 6, no. 1, pp. 14-31, 2019.
[15]   | T. Pan, Z. Wu and A. C. Yip, “Advances in the Green Synthesis of Microporous and Hierarchical Zeolites: A Short Review,” Catalysts, vol. 9, no. 3, p. 274, 2019.
[16]   | C. Kannan, K. Muthuraja and M. R. Devi, “Hazardous dyes removal from aqueous solution over mesoporous aluminophosphate with textural porosity by adsorption,” Journal of Hazardous Materials, Vols. 244-245, pp. 10-20, 2013.
[17]   | K. Muthuraja and C. Kannan, “Kinetic and Isotherm Studies of Removal of Metanil Yellow Dye on Mesoporous Aluminophosphate Molecular Sieves,” Chemical Science Transactions, vol. 2, no. S1, pp. 195-201, 2013.
[18]   | A. B. Albadarin, M. N. Collins, M. Naushad, S. Shirazian, G. Walker and C. Mangwandi, “Activated lignin-chitosan extruded blends for efficient adsorption of methylene blue,” Chemical Engineering Journal, vol. 307, pp. 264-272, 2017.
[19]   | A. W. Burto, K. Ong, T. Rea and I. Y. Chan, “On the estimation of average crystallite size of zeolites from the Scherrer equation: A critical evaluation of its application to zeolites with one-dimensional pore systems,” Microporous and Mesoporous Materials, vol. 117, no. 1-2, pp. 75-90, 2009.
[20]   | G. Leofanti, M. Padovan, G. Tozzola and B. Venturelli, “Surface area and pore texture of catalysts,” Catalysis Today, vol. 41, no. 1-3, pp. 207- 219, 1998.

[21]  
H. Wang, Y. Wang, W. Liu, H. Cai and J. L. J. Liu, “Amorphous magnesium substituted mesoporous aluminophosphate: An acid-base sites synergistic catalysis for transesterification of diethyl carbonate and dimethyl carbonate in fixed-bed reactor,” Microporous and Mesoporous Materials, vol. 292, p. 109757, 2020.

[22]   | M. Shaban, M. R. Abukhadra, M. G. Shahien and S. S. Ibrahim, “Novel bentonite/zeolite-NaP composite efficiently removes methylene blue and Congo red dyes,” Environmental Chemistry Letters, vol. 16, no. 1, pp. 275-280, 2018.
[23]   | T. Huang, M. Yan, K. He, Z. Huang, G. Zeng, A. Chen, M. Peng, H. Li, L. Yuan and G. Chen, “Efficient removal of methylene blue from aqueous solutions using magnetic graphene oxide modified zeolite,” Journal of Colloid and Interface Science, vol. 543, pp. 43-51, 2019.

[24]  
H. Aysan, S. Edebali, C. Ozdemir, M. C. Karakaya, N. K. Aysan, S. Edebali, C. Ozdemir, M. C. Karakaya and N. Karakaya, “Use of chabazite, a naturally abundant zeolite, for the investigation of the adsorption kinetics and mechanism of methylene blue dye,,” Microporous and Mesoporous Materials, vol. 235, pp. 78-86, 2016.

[25]   | I. Shah, R. Adnan, W. Ngah, W. Saime and N. Mohamed, “Iron Impregnated Activated Carbon as an Efficient Adsorbent for the Removal of Methylene Blue: Regeneration and Kinetics Studies,” PLOS ONE, vol. 10, no. 4, pp. 1-23, 2015.
[26]   | T. N. Ramesh, D. V. Kirana, A. Ashwini and T. Manasa, “Calcium hydroxide as low cost adsorbent for the effective removal of indigo carmine dye in water,” Journal of Saudi Chemical Society, vol. 21, no. 2, pp. 165-171, 2017.